Great Thermal Conductivity Enhancement of Silicone Composite with Ultra-Long Copper Nanowires
© The Author(s). 2017
Received: 1 June 2017
Accepted: 16 July 2017
Published: 25 July 2017
In this paper, ultra-long copper nanowires (CuNWs) were successfully synthesized at a large scale by hydrothermal reduction of divalent copper ion using oleylamine and oleic acid as dual ligands. The characteristic of CuNWs is hard and linear, which is clearly different from graphene nanoplatelets (GNPs) and multi-wall carbon nanotubes (MWCNTs). The thermal properties and models of silicone composites with three nanomaterials have been mainly researched. The maximum of thermal conductivity enhancement is up to 215% with only 1.0 vol.% CuNW loading, which is much higher than GNPs and MWCNTs. It is due to the ultra-long CuNWs with a length of more than 100 μm, which facilitates the formation of effective thermal-conductive networks, resulting in great enhancement of thermal conductivity.
KeywordsNanowires Ultra-long Copper Thermal conductivity Silicone composites
Copper is the third most widely used commercial metal (after iron and aluminum) and has received an intensive attention due to its availability and outstanding properties such as good strength, excellent malleability, and superior electrical and thermal conductivity [1–3]. Nowadays, considering their excellent chemical and physical properties and potential applications in electronic devices, more and more attentions have been paid to nanostructures [4, 5]. Nanowires are a kind of one-dimensional nanostructured materials which have high aspect ratio, novel properties, and potential applications [6, 7]. As is known to all, the physical as well as the chemical properties of nanowires depend not only on their native material properties but also on their morphologies and structures. In recent years, newly studied nanowires and their applications include silicon nanowire and copper nanowires, and so on [8, 9]. Among various nanowires, copper nanowires (CuNWs) are one of the hottest one due to their excellent electrical and thermal conductivity. Meanwhile, except for electrical and thermal conductivity, it has been confirmed that the morphology of CuNWs also plays an important role in the performance of polymer composites with CuNWs as functional fillers [10–14].
A number of fabrication methods for CuNWs have been developed, including template-assisted synthesis [15, 16], chemical vapor deposition , vacuum vapor deposition , hydrothermal reduction [13, 14] and so on [19, 20]. However, the above methods are hardly applicable in composite materials because of the limitation in mass production and process complexity. In this paper, large-scale synthesis of ultra-long CuNWs has become a reality through hydrothermal reduction of divalent copper ions using oleylamine and oleic acid as the dual ligands. The CuNWs have been usually used for improving the electrical properties of composite materials [3, 10, 12, 13], but the improvement of composites based on CuNWs was seldom reported. In order to investigate the influence of ultra-long CuNWs on thermal conductivity of polymer composites, silicone composites with different fillers were prepared due to good compatibility of silicone base and easy fabrication of silicone composites. Since graphene nanoplatelets (GNPs) and multi-wall carbon nanotubes (MWCNTs) possess large aspect ratio and superior thermal conductivity [21–24], as a comparison, they were also used for preparing silicone composites. Based on experimental data, the analytical models on polymer composites were developed for simultaneously calculating the thermal property with single or hybrid fillers [25, 26].
Here is a simple method to obtain great thermal conductive silicone composites filled with nanomaterials. There are ultra-long copper nanowires, GNPs, and MWCNTs. It mainly focuses on the morphology features and volume fraction of fillers, which is related to the thermal properties and analytical models of composites. The analysis and comparison of thermal conductivity filled with different fillers are carried out in this work.
Hydrothermal method is widely used to prepare nanowires. Lots of publications have reported this method [27, 28]. Now, the ultra-long CuNWs were also synthesized by this method according to the research of Li et al.  with some modification. Typically, CuCl2·2H2O and glucose were added to H2O under magnetic stirring. Eighty milliliter of oleylamine, 0.8 mL of oleic acid, and 140 mL of ethanol were mixed together. Afterward, these two solutions were put into a beaker and diluted by water, followed by stirring for 12 h at 50 °C. The mixture was transferred into a Teflon-lined stainless steel autoclave. The autoclave was maintained at a temperature of 130 °C for 12 h. The precipitate was sonicated and centrifuged twice in an ethanol solution containing 2.0 wt.% PVP, then vacuum-dried at 50 °C for 6 h.
GNPs were prepared by three steps . Firstly, natural graphite flakes were intercalated by a mixture of concentrated sulfuric and nitric acids (3:1), and then, the intercalated graphite (washed with distilled water and air-dried) was exfoliated by thermal shock on rapid exposure. The exfoliated graphite was dispersed in acetone by high shear mixing for 30 min followed by bath sonication for 24 h. The GNPs were obtained through filtration and drying at 100 °C for 12 h.
The silicone composites with CuNWs were prepared as follows : the CuNWs with different volume fraction were mixed with the silicone base by using a planetary mixer/deaerator (Mazerustar KK-250S, Kurabo, Japan) for 10 min at room temperature. The mixture was further mixed through grinding to obtain silicone composites with different CuNW loading. As a comparison, the silicone composites with different loading of GNPs and MWCNTs (purchased from Chengdu Organic Chemicals Co. Ltd., Chinese Academy of Sciences) were prepared by the same procedure.
The morphologies of different samples were analyzed by a field-emission scanning electron microscope (SEM; S4800, Hitachi, Japan) and a transmission electron microscope (TEM; 2100F, JEOL, Japan). The crystal structure of the samples was characterized by X-ray diffractometer (XRD) (D8 Advance, Bruker, Germany) equipped with a copper target and nickel filter. X-ray wavelength used in the analysis was 0.154 nm of CuKa. The thermal conductivities of the composites were measured by a thermal conductivity analyzer (C-Therm TCi, C-Therm Technologies Ltd., Canada), which is based upon the modified transient plane source principle. The samples were filled into the mold with a thickness of 2 mm. The thermal conductivity of each sample is tested at least five times to obtained average value. The temperature of test system was controlled at 25 °C by constant temperature box (Shanghai Boxun Industry & Commerce Co., Ltd.).
Results and Discussion
The physical properties and aspect ratio of three kinds of fillers
Thermal conductivity (W/mk)
The aspect ratio (SEM and TEM)
Effective aspect ratio (Nielsen model)
For the silicone composites containing CuNWs, the k s and k f are set to 0.12 and 398 W/mK, and it is found that the calculation fits well with the experimental results with A = 186.1, which corresponds to Ar = 350. In the same way, for silicone composites containing GNPs and MWCNTs, the k f are set to 1000 W/mK  and 3000 W/mK , and the calculated results fit well with the experimental results with Ar = 200 and Ar = 100, respectively.
The thermal conductivity of silicone composites containing different fillers depends on the shape, size, and intrinsic thermal conductivity of fillers [30, 36, 37]. It can be seen from Fig. 3 that the thermal conductivity enhancement of silicone composites with CuNWs increases substantially with the increase of the volume fraction than that of silicone composites with GNPs and MWCNTs. The maximum is up to 215% with 1.0 vol.% CuNW loading, much higher than that of silicone nanocomposites with the same GNPs (108%) and MWCNTs (62%) loading. When the volume fraction of fillers is less than 0.5%, the shape, size, and intrinsic thermal conductivity of fillers do not obviously affect the thermal conductivity of silicone composites. This is because the heat-conductive fillers surrounded by silicone base cannot touch each other at low filler loading; hence, the thermal conductivity increases very slowly resulting from high thermal contact resistance inside the composites [30, 36]. While with the loading further increasing, the thermal conductivity of silicone composites with different fillers differs greatly, which indicates that the shape, size, and intrinsic thermal conductivity of fillers have a significant influence on the thermal conductivity improvement of silicone composites. Many studies have reported that the GNPs with superior thermal conductivity and large aspect ratio could greatly improve the thermal conductivity of polymer composites with only a few GNPs [37–39]. And it has stronger ability to enhance the thermal conductivity of polymer composites than MWCNTs [40, 41]. This phenomenon has also been observed in our study. Although the intrinsic thermal conductivity of CuNWs (398 W/mK) is far less than that of GNPs (1000 W/mK) and MWCNTs (3000 W/mK) (as shown in Table 1), the ability of ultra-long CuNWs to enhance the thermal conductivity of silicone composites is stronger than that of GNPs and MWCNTs. It is due to the ultra-long CuNWs with a length of more than 100 μm. The characteristic of CuNWs is hard and linear, which is nothing like MWCNTs (smooth and frizzy). The effective aspect ratio (350) of CuNWs from the Nielsen model is in the range of morphology from SEM and TEM images, which showed the advantage of ultra-long filler on heat transfer. But perhaps because MWCNTs has frizzy and twining structure, the effective aspect ratio (100) from the model is less than that from SEM and TEM. The ultra-long and linear structure facilitates the formation of bridges between themselves and thus to construct some effective thermal conductive networks. These networks provide a low-resistance pathway to heat conduction and increase the overall thermal conductivity of the composite.
In conclusion, a hydrothermal reduction method of divalent copper ions using oleylamine and oleic acid as dual ligands was used to synthesize ultra-long copper nanowires on a large scale. The CuNWs had a diameter of 250~300 nm, a length of more than 100 μm, and an aspect ratio of 333~400, which was observed by scanning electron microscope. The purity and crystal structure of CuNWs was examined by powder X-ray diffraction. Silicone composites with CuNWs, GNPs, and MWCNTs were prepared to investigate the influence of CuNWs on thermal conductivity of polymer composites. The thermal conductivity enhancement of silicone composite with ultra-long CuNWs increases substantially with the increase of the volume fraction. The maximum is up to 215% with 1.0 vol.% CuNW loading, much higher than that of silicone nanocomposites with the same GNP (108%) and MWCNT (62%) loading. It is due to the ultra-long length and large aspect ratio, which facilitates the formation of effective thermal conductive networks, resulting in great enhancement of thermal conductivity.
The work was supported by the National Natural Science Foundation of China (51476094 and 51590902) and the key subject of Shanghai Second Polytechnic University (No. 4, Material Science, XXKPY1302).
WY proposed the idea and provided some supporting about the experiments and analysis. LZ completed most of the experiments with JY, and they were both involved in drafting the manuscript. MW completed part of the experiments. HX provided some supporting about the work, and he helped to revise the manuscript and gave other authors some suggestions. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Papp JF (2008) U.S. Geological Survey, Mineral Commodity Summaries. J Chem Inf Model 53(703):160Google Scholar
- Groza JR, Gibeling JC (1993) Principles of particle selection for dispersion-strengthened copper. Mater Sci Eng A 171(1–2):115–125View ArticleGoogle Scholar
- Lin B, Gelves AG, Haber JA, Sundararaj U (2007) Electrical, rheological, and mechanical properties of polystyrene/copper nanowire nanocomposites. Ind Eng Chem Res 46(8):2481–2487View ArticleGoogle Scholar
- Rao CNR, Deepak FL, Gundiah G, Govindaraj A (2003) Inorganic nanowires. Prog Solid State Chem 31(1–2):5–147View ArticleGoogle Scholar
- Xia Y, Yang P, Sun Y, Wu Y, Mayers B, Gates B et al (2003) Synthesis, characterization, and applications. Adv Mater 15:353–389View ArticleGoogle Scholar
- Jiang Y, Xiu G, Qin R, Liu H, Xia C, Ma H (2016) Efficiency enhancement mechanism for poly(3,4-ethylenedioxythiophene):poly(styrenesulfonate)/silicon nanowires hybrid solar cells using alkali treatment. Nanoscale Res Lett 11(1):267View ArticleGoogle Scholar
- Zeng JL, Zhu FR, Yu SB, Zhu L, Cao Z et al (2012) Effects of copper nanowires on the properties of an organic phase change material. Sol Energ Mat Sol C 105(105):174–178View ArticleGoogle Scholar
- Wang F, Gao Y, Zhu T, Zhao J (2011) Shock-induced breaking of the nanowire with the dependence of crystallographic orientation and strain rate. Nanoscale Res Lett 6(1):291View ArticleGoogle Scholar
- Guerfi Y, Larrieu G (2016) Vertical silicon nanowire field effect transistors with nanoscale gate-all-around. Nanoscale Res Lett 11(1):210View ArticleGoogle Scholar
- Silva ABD, Arjmand M, Sundararaj U et al (2014) Novel composites of copper nanowire/PVDF with superior dielectric properties. Polymer 55(1):226–234View ArticleGoogle Scholar
- Li S, Chen Y, Huang L et al (2014) Large-scale synthesis of well-dispersed copper nanowires in an electric pressure cooker and their application in transparent and conductive networks. Inorg Chem 53(9):4440View ArticleGoogle Scholar
- Tang Y, Kai LY, Chen Y et al (2013) Ultralow-density copper nanowire aerogel monoliths with tunable mechanical and electrical properties. J Mater Chem A 1(23):6723–6726View ArticleGoogle Scholar
- Cheng Y, Wang S, Wang R (2014) Copper nanowire based transparent conductive films with high stability and superior stretchability. J Mater Chem C 2(27):5309–5316View ArticleGoogle Scholar
- Wang S, Cheng Y, Wang R et al (2014) Highly thermal conductive copper nanowire composites with ultralow loading: toward applications as thermal interface materials. ACS Appl Mater Interfaces 6(9):6481–6486View ArticleGoogle Scholar
- Toimil Molares ME, Hohberger EM, Schaeflein C et al (2003) Electrical characterization of electrochemically grown single copper nanowires. Appl Phys Lett 82(13):2139–2141View ArticleGoogle Scholar
- Kudo H, Fujihira M (2006) DNA-templated copper nanowire fabrication by a two-step process involving electroless metallization. IEEE Trans Nanotechnol 5(2):90–92View ArticleGoogle Scholar
- Choi H, Park SH (2004) Seedless growth of free-standing copper nanowires by chemical vapor deposition. J Am Chem Soc 126(20):6248–6249View ArticleGoogle Scholar
- Liu Z, Bo Y (2003) A novel method for preparing copper nanorods and nanowires. Adv Mater 15(4):303–305View ArticleGoogle Scholar
- Rathmell AR, Bergin SM, Hua YL et al (2010) The growth mechanism of copper nanowires and their properties in flexible, transparent conducting films. Adv Mater 22(32):3558View ArticleGoogle Scholar
- Duan JL, Liu J, Yao HJ et al (2008) Controlled synthesis and diameter-dependent optical properties of Cu nanowire arrays. Mat Sci Eng B 147(1):57–62View ArticleGoogle Scholar
- Rao CNR, Sood AK, Subrahmanyam KS, Govindaraj A (2009) Graphene: the new two-dimensional nanomaterial. Angew Chem Int Edit 48:7752View ArticleGoogle Scholar
- Balandin AA, Ghosh S, Bao W et al (2008) Superior thermal conductivity of single-layer graphene. Nano Lett 8(3):902View ArticleGoogle Scholar
- Balandin AA (2011) Thermal properties of graphene, carbon nanotubes and nanostructured carbon materials. Nat Mater 10(8):569–581View ArticleGoogle Scholar
- Pop E, Mann D, Wang Q et al (2005) Thermal conductance of an individual single-wall carbon nanotube above room temperature. Nano Lett 6(1):96–100View ArticleGoogle Scholar
- Chen L, Sun YY, Xu HF et al (2016) Analytic modeling for the anisotropic thermal conductivity of polymer composites containing aligned hexagonal boron nitride. Compos Sci Technol 122:42–49View ArticleGoogle Scholar
- Chen L, Sun YY, Lin J et al (2015) Modeling and analysis of synergistic effect in thermal conductivity enhancement of polymer composites with hybrid filler. Int J Heat Mass Tran 81:457–464View ArticleGoogle Scholar
- Wang M, Li S, Zhang P et al (2015) A modified sequential method used to prepare high quality perovskite on ZnO nanorods. Chem Phys Lett 639:283–288View ArticleGoogle Scholar
- Li S, Zhang P, Chen H et al (2017) Mesoporous PbI2, assisted growth of large perovskite grains for efficient perovskite solar cells based on ZnO nanorods. J Power Sources 342:990–997View ArticleGoogle Scholar
- Chatterjee S, Wang JW, Kuo WS et al (2012) Mechanical reinforcement and thermal conductivity in expanded graphene nanoplatelets reinforced epoxy composites. Chem Phys Lett 531(13):6–10View ArticleGoogle Scholar
- Yu W, Zhao J, Wang M et al (2015) Thermal conductivity enhancement in thermal grease containing different CuO structures. Nanoscale Res Lett 10(1):1–8View ArticleGoogle Scholar
- Cao A, Xu C, Liang J et al (2001) X-ray diffraction characterization on the alignment degree of carbon nanotubes. Chem Phys Lett 344(1):13–17View ArticleGoogle Scholar
- Chen CM, Dai YM, Huang JG et al (2006) Intermetallic catalyst for carbon nanotubes (CNTs) growth by thermal chemical vapor deposition method. Carbon 44(9):1808–1820View ArticleGoogle Scholar
- Nielsen LE (1974) Thermal and electrical-conductivity of 2-phase systems. Ind eng Chem Fundam 13(1):17Google Scholar
- Murali R, Yang Y, Brenner K et al (2009) Breakdown current density of graphene nanoribbons. Appl phys Lett 94(24):243114-243114-3Google Scholar
- Kim P, Shi L, Majumdar A et al (2001) Thermal transport measurements of individual multiwalled nanotubes. Phys Rev Lett 87(21):215502View ArticleGoogle Scholar
- Zhou WY, Qi SH, Zhao HZ et al (2007) Thermally conductive silicone rubber reinforced with boron nitride particle. Polym Composite 28(1):23–28View ArticleGoogle Scholar
- Yu W, Xie H, Chen L et al (2014) Graphene based silicone thermal greases. Phys Lett A 378(3):207–211View ArticleGoogle Scholar
- Yu A, Ramesh P, Itkis ME et al (2007) Graphite nanoplatelet—epoxy composite thermal Interface materials. J Phys Chem C 111(21):084504–084504-4Google Scholar
- Shahil KM, Balandin AA (2012) Graphene-multilayer graphene nanocomposites as highly efficient thermal interface materials. Nano Lett 12(2):861View ArticleGoogle Scholar
- Yu A, Ramesh P, Sun X et al (2008) Enhanced thermal conductivity in a hybrid graphite Nanoplatelet-carbon Nanotube filler for epoxy composites. Adv Mater 20(24):4740–4744View ArticleGoogle Scholar
- Yang SY, Lin WN, Huang YL et al (2011) Synergetic effects of graphene platelets and carbon nanotubes on the mechanical and thermal properties of epoxy composites. Carbon 49(3):793–803View ArticleGoogle Scholar